Inorg. Chem. 1990, 29, 4059-4062 reducing agent other than CO, e.g. Zn, which can also serve as a chloride acceptor. If structure 2a is correct for the adsorbed tricarbonyl on SiOz and N a y , then there should be no reaction between the adsorbed carbonyl chloride and C O a t room temperature, since there is nothing that can serve as a chloride acceptor. This is indeed the case; no reaction is observed between 2a and C O (25 O C , 1 atm) after 24 h. Similarly, a reaction is to be expected between 2b on MgO and C O at room temperature. Although a reaction does occur, it is unfortunately not nearly as clean as previously observed on A1203. Thus, when 2b on MgO is treated with CO, a very complicated infrared spectrum is obtained. Some of the bands may be due to [ H R ~ ~ ( C 0 ) ~ , ] - ( a dbut s ) ,if this anion is present, it is not the major product. That a reaction takes place a t all however is consistent with MgO acting as a chloride acceptor. Conclusion Although R u ( C O ) ~ C I ~ ( T H Fis) spontaneously adsorbed by a
number of oxides, it is impossible to determine the surface structure of the adsorbed species simply by the infrared spectrum. Thus, a previous study on silica assigned the surface structure as Ru"(CO),(ads), a structure that does not contain coordinated chloride. It is apparent from the present study that a better description of the surface carbonyl on Si02and N a Y zeolite is Ru(CO),Cl,(ads). Only on the more basic oxides, Al2O3 and MgO, is chloride lost to yield the surface species R ~ ~ I ( C 0 ) ~ ( a d s ) . It is further proposed that the surface ligands include two oxides, 0-AI, so that the adsorbed tricarbonyl is not a formally cationic complex. Importantly, the distinction between the two surface structures is not readily made simply from the infrared spectra. The basic chemical reactions of the adsorbed carbonyls are required to confirm the proposed structures. Acknowledgment. Support for this work was provided by the National Science Foundation (Grant D M R 85-18364). B.E.H. acknowledges an A. von Humboldt fellowship during part of this work.
Contribution from the Department of Chemistry, Cornell University, Ithaca, New York 14853
Synthesis, Structure, and Properties of a New Ternary Metal Nitride, Ca3CrN3 Deborah A. Vennos, Michael E. Badding, and F. J. DiSalvo* Received February 27, 1990 We have synthesized a new ternary nitride, Ca,CrN,, from the binary nitrides at high temperature. The refined structure was solved in the Cmcm space group, Z = 4, with lattice constants (A) a = 8.503 (2), b = 10.284 (2), and c = 5.032 ( I ) and with R = 3.9% and R, = 3.9%. This new structure type consists of sheets of [CrN3I6 planar triangular units and calcium ions. Ca3CrN3 is insulating and paramagnetic with Cr3+in the low-spin state. This is the first unambiguous example of low-spin Cr3+. Larger than expected antiferromagnetic interactions produce a maximum in the magnetic susceptibility at 240 K, even though the shortest Cr-Cr distance is 4.73 A.
Introduction Although the chemistry of binary nitrides has been explored in detail, comparatively little work on ternary and quaternary nitrides has been reported. Preliminary work has shown that, in addition to the facile formation and stability of ternary nitrides containing electropositive elements, these phases exhibit a variety of novel properties. Examples include the N i d9 configuration in CaNiN,] the layered structures of MTaN? (M = alkali metal), and the unique structure types found in CazlFe3N17,3 Li3AINz,4 and CaGaN.5 These few examples suggest that ternary nitrides will display an extensive assortment of new compounds and structure types. We therefore undertook a large-scale investigation of alkaline-earth-metal- and transition-metal-containing nitrides. Herein, we report a new compound and structure type, Ca,CrN,, discovered initially as an impurity phase in reactions of Ca3N2 in stainless steel containers. Experimental Section Starting Materials. Chromium nitride was prepared by heating Cr powder (-100 mesh, 3N) in flowing nitrogen (prepurified by passing through finely divided copper at 150 "C and then activated alumina) at 800 "C for 1 day. The product was ground and reheated several times, yielding a mixture of CrN and Cr,N (approximately 50:SO). Granules of calcium (2N) were reacted at 1000 OC for 3 days in flowing nitrogen
The compound was then prepared as a majority phase by heating 0.2048 g of the CrN/Cr,N mixture (1.11 mmol of the hypothetical Cr,N2) and 0.601 1 g of Ca3N, (4.06 mmol) in a sealed stainless steel tube under an argon atmosphere at 1350 OC for 4 days, followed by cooling to 1050 "C in 5 h and finally cooling to room temperature in 12 h. There was no evidence of Ca3Nzremaining in the product mixture;
however, the brittle nature of the once malleable tube indicated that the excess Ca3Nzwas consumed by a reaction with the stainless steel. The product contained air-sensitive, burgundy needle crystals up to 1 mm in length, which were used for the structure determination. X-ray powder diffraction indicated a nearly pure Ca3CrN3 powder with a small unidentified impurity phase. The intensity of the strongest impurity diffraction peak was 6% as intense as the strongest peak of the majority
The material used for susceptibility measurements was prepared by heating a pressed pellet of an intimate mixture of 0.3103 g of CrN/Cr2N (1.69 mmol of Cr3N,) and 0.5070 g of CapNz(3.43 mmol) powders in a sealed molybdenum crucible under argon at the heating schedule mentioned above. The only impurity observable in the product by powder X-ray diffraction was Cr metal. The most intense Cr peak was only 6%
Chern, M. Y.; DiSalvo. F. J. Submitted for publication in J . Solid Sfate Chem. Jacobs, H.; von Pinkowski, E. J . Less-Common M e t . 1989, 146, 147. Verdier, P.; Marchand, R.; Lang, J . Rev. Chim. Miner. 1976, 13, 214. Juza, V. R.;Hund, F. 2. Anorg. Allg. Chem. 1948, 257, 13. Verdier, P.; L'Haridon, P.; Maunaye. M.; Marchand, R. Acfa Crysmllogr. 1914, 30, 226. I
(prepurified as above) to yield pure Ca3Nz. The binary products were identified by X-ray powder diffraction methods. Since both Ca3N2and Ca,CrN3 are air sensitive, all manipulations were carried out in an argon-filled glovebox. Synthesis of Ca3CrN,. The title compound was first discovered as a minority crystalline phase in a reaction of Ca3Nzand tin in a stainless steel tube. The bulk phase consisted of a gray powder, Ca3SnN,6with a minority phase consisting of needle crystals distributed throughout. Microprobe analysis of the crystals indicated the presence of calcium and chromium (a component in the stainless steel) at a Ca:Cr molar ratio of
( 6 ) Chern, M. Y . ; Vennos, D. A.; DiSalvo, F. J . To be published. 1
0 1990 American Chemical Society
Vennos et al.
4060 Inorganic Chemistry, Val. 29, No. 20, 1990
w' ' I '~ ' ' 1 Table 11. '
Positional Parameters for Ca,CrN, atom site X Y Ca 4c 0 0.1079 12) Ca 8g 0.2843 (2) -0.1174 ( i j 0.1945 (2) Cr 4c 0.5 N 4c 0.5 0.3757 (8) 0.1286 (6) 0.6918 (8) N 8g
0.25 0.25 0.25 0.25 0.25
Figure 1. Temperature dependence of the magnetic susceptibility of Ca3CrN1. Table 1. Summary of Crystal and Diffraction Data for Ca,CrN, space group Cmem (No. 63)
a. b, e.
cryst dimens. mm 20 m ,a?. deg; scan type octants measd X-ray radiation monochromator no. of measd reflcns no. of obsd reflcns' no. of independent reflcns abs coeff AL, mm-' R,b Rw: %
4 8.503 (2). 10.284 (2). 5.032 ( I ) 440 0.113 x 0.04 x 0.13 55; w-20 &h,k.l
Mo Ka graphite 577 303 263 5.79 3.9, 3.9
as intense as the strongest Ca3CrN3peak. Since the lower symmetry of Ca3CrN3splits the X-ray lines into many components, the impurity level of Cr was estimated to be less than 3 wt %. A larger percentage of Cr from the reaction mixture should have remained in the product; most of it must have alloyed with the molybdenum crucible, as it is not observed in the product. Magnetic Susceptibility. The magnetic susceptibility of the sample was measured by the Faraday technique in a previously calibrated system.' The susceptibility ofa sample sealed in a thin-walled quartz tube was determined to be field independent at room temperature, showing that no ferromagnetic impuritie-s were present. Figure I shows the results of a temperature-dependent study between 30 and 750 K at a magnetic field strength of 14.2 kC. The contribution of the <3 wt % Cr impurity to the observed peak in the susceptibility is negligible. since its gram susceptibility is approximately 3 X IOd emu/g and weakly temperature dependent, increasing by only 10% from 0 to 800 K.8 Electrical Properties. The resistance of a pellet of Ca,CrN, was measured in a small press inside the glovebox. The two pistons were electrically insulated from each other. allowing a two-point measurement of the resistance. The resistance determined on a pellet 4.5 mm in diameter and approximately 3 mm thick was 45 kR. Structure Determination. Unit cell symmetry and approximate lattice constants were obtained from Weissenberg photographs of a crystal mounted along the needle axis. A 0.03 X 0.04 X 0.13 mm' crystal, sealed in a glass capillary under argon, was used in the structure determination. Data were collected on a Syntex P2, diffractometer using Mo K a radiation and a graphite monochromator. The choice of space groups was reduced to Cmcm, Cmc2,. and C2cm by systematic absences, and the Structue was salved by using direct methods in the Cmem space group. Refinement in either noncentrasymmetric space group resulted in no
Figure 2. View of the str~cturedawn the (1 axis. The Ca atoms are open circles, Cr atoms are dotted circles. and N atoms are partially hatched circles
Vasiliou. 1.;Hornbostel, M.; Ziebarth. R.; DiSalvo, F. J. J. SolidSrore
Chem. 1989,81, 208. (8) Vogt, E.: Hahl. M.Zahlenwerte und Funkrimen (1"s Physik Chemie Landalt, Bornstein, Ws.; Asrronomie Geophysik Technik. 6th 4.; Springer-Verlag: Berlin, 1962: Vol. 2, pp 1-8.
Figure 3. View of Ca,CrN, dawn the e axis, showing one unit cell and indicating the labels used to identify the atoms in Table 111. significant change in the structure or R factors. An empirical absorption correction (the $--scan method) was performed, and two Octants of data were collected and merged to improve the data set. The largest peak in the final difference Fourier map was 0.86 e. Final R = 3.9% and R. = 3.9% were obtained after refinement. The structure determination and refinement were performed by using Nicolet SHELXTL Plus software running on a Microvax computer. Table I summarizes data collection parameters. Atomic positions are listed in Table 11. After the structure was solved, the powder patterns taken on a Scintag XDS2000 diffractometer could be indexed. The observed patterns matched that calculated by Lazy Pulverix? on the basis of the singlecrystal data.
Results and Discussion The structure of Ca,CrN, (Figures 2 a n d 3) consists of triangular [CrN3I6- units with C,, point symmetry separated by calcium atoms (the C, axis is parallel to the b axis). A view down the a axis clearly shows the sheet structure of the planar groups and the intervening Ca atoms. In each sheet the triangular units are pointing in the same direction. Neighboring sheets are displaced by 'I2in z, and the orientation of the triangles is reversed. A list of relevant bond distances and angles can be found in Table 111. Although the triangular planar coordination of a transition metal by nitrogen has been observed in molecular solids,'OJ' this (9) Yvon, K.; Jeitschko, W.; Parthe, E. J. Appl. Crysrollogr. 1977, IO. 73. (10) Bradley, D. C.; Chisholm. M. H. Ace. Chem. Res. 1976, 9, 273.
Inorganic Chemistry, Vof. 29, No. 20, 1990 4061
Figure 4. (a) Distorted octahedral environment of the unique nitrogen atomI (N(lc)). (b) Coordination about the equivalent nitrogen atoms (N(la), N(lb)). (c) Local environment about the unique calcium atom (Ca(1a)). (d) Irregular coordination about the equivalent calcium atoms (Ca(2a), Ca( 2c)).
Table 111. Important Distances (A) and Angles (deg) in Ca,CrN, Nonbonding Interactions Cr(l).-Cr(2) 5.032 ( I ) Ca(lb)...Ca(4b) 3.349 (2) Ca(Zb)...Ca(Zc) 3.368 (3) Cr(l)...Cr(3) 4.726 (I)’ Cr(l)...Ca(la) 3.234 (2) Ca(2b)...Ca(3a) 3.491 (I)“ Cr(l)...Ca(lb) 3.234 (2) Ca(Za)...Ca(Zc) 3.668 (4) Cr(l)-.Ca(3a) 3.213 ( 1 ) O Ca(2a)..Ca(3a) 3.757 (2) Cr(4)..Ca(2a) 3.695 (2) Ca(Za)...Ca(4b) 3.487 (2) Ca(lb)..Ca(3b) 3.355 (3) Cr(l)-N(lb) Cr(l)-N(la) Cr(l)-N(lc) Ca(la)-N(lc) Ca(1b)-N(lc) N(la)-Cr(1)-N(lc) N(1b)-Cr(1)-N(1c)
Bonding Interactions 1.766 (7) Ca(2a)-N(lc) Ca(2a)-N(lb) 1.766 ( 7 ) 1.864 (8) Ca(2b)-N(lb) 2.522 (1) Ca(3b)-N(lc) Ca(4a)-N(2a) 2.522 ( I ) Bond Angles 112.6 (2) N(1b)-Cr(1)-N(1a) 112.6 (2)
2.419 (2) 2.728 (6) 2.629 (7) 2.388 (8) 2.538 (6) 134.9 (4)
“Distance indicated is from an atom in the unit cell shown to an atom in an adjacent unit cell, respectively.
is the first example of such coordination in the solid state. The coordination geometry around the nitrogens is a distorted octahedron, consisting of four “equatorial” Ca’s, one “axial” Ca, and one “axial” Cr. The bond lengths about the unique N (N(1c) in Figures 3 and 4a) are 2 X 2.522 A, 2 X 2.419 A, and 2.388 A ( I I ) Bradley, D. C.; Hursthouse, M.9.; Newing, C. W. Chem. Commun. 1971, 8, 41 1.
to Ca and 1.864 A to Cr. The two equivalent nitrogens (N( l a ) and N(1b) in Figures 3 and 4b) have similar bond lengths, but the octahedral angles are considerably distorted from 90°, and the Cr-N bond lengths are compressed to 1.766 A. The environment about the unique calcium (Ca( l a ) in Figures 3 and 4c) can be approximated as a square pyramid of nitrogens with two additional long Ca-Cr bonds. However, the environment about the two equivalent calciums (Ca(2a) and Ca(2c) in Figures 3 and 4d) is quite irregular with 6-fold coordination to nitrogen. There are very few compounds with Cr-N bonds with which to compare distances. The Cr-N bond lengths in molecular solids range from a Cr-N formal triple bond (1.57 A)lz to apparent single bonds in the range 2.04-2.25 A.13-19 In the solid state, Cr-N bond lengths average considerably larger (2.06-2.93 A).*z The Cr-N distances in the [CrN3I6 unit indicate multiple metal (12) Groves, J. T.; Takahashi, T.; Butler, W. M. Inorg. Chem. 1983, 22, 884. (13) Bush, M. A,; Sim, G. A. J . Chem. SOC.A 1970, 4, 605. (14) Greenhough,T. J.; Kolthammer, B. W.; Legzdins, P.; Trotter, J. Inorg. Chem. 1979, 18, 3548. (15) Bino, A.; Cotton, F. A.; Kaim, W. Inorg. Chem. 1979, 18, 3566. (16) Richeson, D. S.;Mitchell, J . F.; Theopold, K. H. Organometallics 1989, 8, 2570. (17) Ball, R. G.; Hames, B. W.; Legzdins, P.; Trotter, J. Inorg. Chem. 1980, 19, 3626. (18) Albrecht, V. G. Z. Chem. 1963, 3, 182. (19) Ford, P. D.; Larkworthy, L. F.; Povey, D. C.; Roberts, A. J. Bull. Soc. Chim. Fr. 1983, 2, 1983. (20) Aivazov, M. 1.; Rezchikova, T. V. Russ. J . Inorg. Chem. (Engl. Transl.) 1977, 22, 250. (21) Eddine, M. N.; Bertaut, E. F.;Roubin, M.; Paris, J. Acta Crystallogr., Secf. B 1977, 338, 3010. (22) Juza, R. V.; Jurgen, H. Z . Anorg. Allg. Chem. 1961, 309, 276.
4062 Inorganic Chemistry, Vol. 29, No. 20, 1990 to nitrogen bonding in comparison to the average Cr-N single bond distances in molecular solids. The closest Ca-Ca distance between the planar units (3.36 A) is slightly longer than that in Ca3N (3.16 A).23 However, the closest Ca-N distances (2.38, are similar to those in Ca3N2(2.46 A),23Ca3BiN (2.45 2.54 A),6 and CaNiN (2.50 A).] The Cr-Cr distances are much too long for any metal-metal bonding or significant direct exchange interactions. The shortest distance, 4.73 A, is between Cr in adjacent sheets (Cr(1) or Cr(2) to Cr(3) in the unit cell below the one shown in Figure 3). The next closest distances are 5.03 A (Cr(1) to Cr(2), across two sheets) and 5.06 A (Cr(3) to Cr(4) in Figure 3). These long Cr-Cr distances suggest a very small exchange interaction between paramagnetic Cr3+ ions. Consequently, we expected the susceptibility to follow a simple Curie-Weiss law, where the susceptibility is equal to C/( T 0) and 0 is expected to be less than I O K. W e ignore the small temperature-independent term expected in the susceptibility, since it is a sum of a small diamagnetic term (the core diamagnetism, between -0.2 X IOd and -0.33 X 10” depending upon the poorly established value of the core diamagnetism for N in solids) and a small paramagnetic term (the van Vleck paramagnetism, which is unknown). The fact that the susceptibility does not follow the simple Curie-Weiss law (at least below approximately 400 K) suggests that strong antiferromagnetic superexchange interactions must follow paths such as Cr-N-N-Cr or Cr-N-Ca-N-Cr. The lack of a sharp break in the susceptibility implies that three-dimensional long-range order of the Cr spins does not occur above 30 K . The broad peak in the susceptibility therefore suggests moderately strong antiferromagnetic interactions in only one or two dimension^.^^ Since the optimal exchange pathways are not obvious, it is not possible to be certain about the dimensionality of the exchange interactions. However, if the dominant exchange is between closest neighbor Cr atoms, then the exchange pathway forms a zigzag chain parallel to the c axis. The next closest Cr-Cr distances are only 0.3 A longer; consequently, our assignment of the optimal exchange path may not be correct. In principle, the magnetic susceptibility can be used to determine the spin of the Cr. Since the Cr site symmetry is so low, none of the Cr d states are degenerate. Depending upon their relative splittings, the Cr3+ could be high spin (S = 3/2) or low spin (S = I,/*). If the exchange is Heisenberg-like and one-dimensional, the product of the molar susceptibility at the maximum and the
(23) Laurent, Y.; Lang, J.; LeBihan, M. T. Acra Crystallogr.,Secr. B 1968, 248, 494. (24) Selwood, P. W. Magnelochemistry; Wiley Interscience: New York, 1979. ( 2 5 ) Hatfield, W. E. I n Solid State Chemistry: Techniques; Cheetham, A. K..Day, P., Eds.; Oxford Science Publications: London, 1987; Chapter 4.
Vennos et al. temperature of the maximum is a function only of the spin.25 The maximum molar susceptibility is 6.85 X 1 O-” emu/mol, and the temperature at the maximum is 240 K. The product, 0.164 emu.K/mol, is close to that expected for S = (0.141 emu. K/mol) but much smaller than that expected for S = 3 / 2 (0.648 e m ~ . K / m o l ) . * Since ~ the experimental value is not exactly equal to the theoretical number for S = other exchange pathways may also be important. At very high temperatures the effective moment per Cr theoretically must extrapolate to the free ion value. At the highest temperature of measurement we obtain 1.86 pB,somewhat above the expected infinite temperature pin-'/^ value of 1.73 pB but considerably below the pin-^/^ value of 3.87 pB. The source of the small discrepancy is not clear but could be caused by a van Vleck susceptibility that is larger than the core diamagnetism or by a small thermal population of the excited pin-^/^ state. In any case, the spin state of Cr3+in this compound is clearly low-spin s = ]I2. The exchange energy, J, is also obtainable from the temperature of the maximum.25 We obtain J = 185 f 5 K. It is surprising to us that such a large exchange can occur between paramagnetic centers almost 5 A apart. This is likely due to a large covalent contribution to the bonding and overlaps from one Cr to the next, although we did not expect the exchange to be so large, as previously discussed. To our knowledge this is the first unambiguous example of a low-spin Cr3+ compound. One previous publication26 on chromium-doped silicates suggests that chromium occupies both octahedral and tetrahedral sites and that the tetrahedrally coordinated Cr3+ is low spin, but we could find no references to a concentrated chromium compound that contained such low-spin species. To summarize, the new phase Ca3CrN3has been prepared by reaction of the binary nitrides at high temperature. The compound represents a new structure type, consisting of triangular planar [CrN3I6-units separated by calcium atoms. It is a paramagnetic insulator with low-spin Cr3+ and low-dimensional antiferromagnetic interactions. Acknowledgment. We wish to extend appreciation to Greg VanDuyne of the Cornell Chemistry X-ray Facility for assistance with the structure determination. D.A.V. would like to express gratitude to Ming Y. Chern for his generous help in getting started with the nitrides. Support of this work through the Office of Naval Research is greatly appreciated. Supplementary Material Available: For Ca,CrN,, a table of refined anisotropic thermal parameters (1 page); a table of observed and calculated structure factors (1 page). Ordering information is given on any current masthead page. (26)
Ikeda, K . Kobutsugaku Zasshi 1984, 16 (9,385.